CARBON NANOTUBES AND RELATED STRUCTURES New Materials for the Twenty-ﬁrst Century
Peter J. F. Harris Department of Chemistry, University of Reading The Pitt Building, Trumpington Street, Cambridge, United Kingdom The Edinburgh Building, Cambridge CB2 2RU, UK www.cup.cam.ac.uk 40 West 20th Street, New York, NY 10011-4211, USA www.cup.org 10 Stamford Road, Oakleigh, Melbourne 3166, Australia Ruiz de Alarco´ n 13, 28014 Madrid, Spain
© Cambridge University Press 1999
This book is in copyright. Subject to statutory exception and to the provisions of relevant collective licensing agreements, no reproduction of any part may take place without the written permission of Cambridge University Press.
First published 1999
Printed in the United Kingdom at the University Press, Cambridge
Typeset in Times 11/14pt 
A catalogue record for this book is available from the British Library
Library of Congress Cataloguing in Publication data Harris, Peter J. F. (Peter John Frederich), 1957— Carbon nanotubes and related structures: new materials for the 21st century/Peter J. F. Harris. p. cm. Includes bibliographical references. ISBN 0 521 55446 2 (hc.) 1. Carbon. 2. Nanostructure materials. 3. Tubes. I. Title. TA455.C3H37 1999 620.193—dc21 99-21391 CIP
ISBN 0 521 55446 2 hardback Contents
Acknowledgements page xiii
1 Introduction 1 1.1 The discovery of fullerene-related carbon nanotubes 3 1.2 Characteristics of multiwalled nanotubes 4 1.3 Single-walled nanotubes 7 1.4 Pre-1991 evidence for carbon nanotubes 10 1.5 Nanotube research 12 1.6 Organisation of the book 13 References 14
2 Synthesis: Preparation methods, growth mechanisms and processing techniques 16 2.1 Production of multiwalled nanotubes: non-catalytic methods 18 2.1.1 The arc-evaporation technique 18 2.1.2 The quality of nanotube samples produced by arc-evaporation 21 2.1.3 Safety considerations 21 2.1.4 Condensation of carbon vapour in the absence of an electric ﬁeld 22 2.1.5 Pyrolytic methods 23 2.1.6 Electrochemical synthesis of nanotubes 24 2.2 Experiments on the heat treatment of fullerene soot 25 2.3 Catalytically produced multiwalled nanotubes 28 2.3.1 Background 28 2.3.2 Growth mechanisms of catalytically produced nanotubes 30 2.3.3 Synthesis of aligned nanotubes by catalysis 34
vii viii Contents 2.4 Nanotubes on TEM support grids: a word of warning 34 2.5 Single-walled nanotubes 37 2.5.1 Discovery 37 2.5.2 Subsequent work on single-walled tubes 39 2.5.3 Nanotube ‘ropes’ 41 2.6 Theories of nanotube growth 43 2.6.1 General comments 43 2.6.2 Why do tubes remain open during growth? 44 2.6.3 Properties of the arc plasma 45 2.6.4 An alternative model 46 2.6.5 Growth of single-walled nanotubes 47 2.7 Puriﬁcation of multiwalled tubes 49 2.8 Puriﬁcation of single-walled tubes 52 2.9 Alignment of nanotube samples 53 2.10 Length control of carbon nanotubes 53 2.11 Discussion 54 References 56
3 Structure 61 3.1 Classiﬁcation of tubular biological structures 62 3.2 Bonding in carbon materials 65 3.3 The structure of carbon nanotubes: theoretical discussion 66 3.3.1 Vector notation for carbon nanotubes 66 3.3.2 Unit cells of nanotubes 68 3.3.3 Multiwalled nanotubes 71 3.3.4 Theory of nanotube capping 72 3.3.5 Symmetry classiﬁcation of nanotubes 75 3.3.6 Elbow connections, tori and coils 78 3.3.7 Arrays of single-walled nanotubes 79 3.4 The physical stability of carbon nanotubes 82 3.5 Experimental studies of nanotube structure: multiwalled nanotubes 82 3.5.1 Techniques 82 3.5.2 The layer structure: experimental observations 83 3.5.3 The layer structure: models 85 3.5.4 Electron diﬀraction 88 3.5.5 Plan-view imaging by HREM 89 3.5.6 The cross-sectional shape of multiwalled nanotubes 91 3.5.7 HREM studies of cap structure 92 3.5.8 Elbow connections and branching structures 95 Contents ix 3.6 Experimental studies of nanotube structure: single-walled nanotubes 98 3.6.1 High resolution electron microscopy and electron diﬀraction 98 3.6.2 Scanning probe microscopy 99 3.6.3 Nanotube hoops and diameter doubling 100 3.7 Structure of carbon nanoparticles 102 3.8 Nanocones 104 3.9 Discussion 105 References 107
4 The physics of nanotubes 111 4.1 Electronic properties of graphite and carbon ﬁbres 112 4.1.1 Band structure of graphite 112 4.1.2 Transport properties of graphite, disordered carbons and carbon ﬁbres 114 4.1.3 Magnetoresistance of graphite and carbon ﬁbres 114 4.2 Electronic properties of nanotubes: theory 115 4.2.1 Band structure of single-walled tubes 115 4.2.2 Band structure of multiwalled tubes 120 4.2.3 Electron transport in nanotubes 120 4.2.4 Nanotube junctions 121 4.2.5 Electronic properties of nanotubes in a magnetic ﬁeld 121 4.3 Electronic properties of nanotubes: experimental measurements 123 4.3.1 Resistivity measurements on multiwalled nanotubes 123 4.3.2 Resistivity measurements on single-walled nanotubes 130 4.3.3 Doping of nanotube bundles 134 4.3.4 Electron spin resonance 134 4.4 Magnetic properties of nanotubes 137 4.5 Optical properties of nanotubes 140 4.6 Vibrational properties of nanotubes 141 4.6.1 Symmetry of vibrational modes 141 4.6.2 Experimental IR and Raman spectra: multiwalled nanotubes 144 4.6.3 Experimental IR and Raman spectra: single-walled nanotubes 144 4.7 Electron energy loss spectroscopy of nanotubes 147 4.8 Nanotube ﬁeld emitters 149 4.9 Discussion 150 References 151 x Contents 5 Nanocapsules and nanotest-tubes 156 5.1 Metallofullerenes 157 5.2 Filling nanotubes and nanoparticles by arc-evaporation 158 5.2.1 Early work 158 5.2.2 Further studies 158 5.3 Preparation of ﬁlled nanoparticles from microporous carbon 162 5.4 Properties of ﬁlled nanoparticles 164 5.4.1 Protection from environmental degradation 164 5.4.2 Encapsulation of magnetic materials 164 5.4.3 Encapsulation of radioactive materials 165 5.5 Technegas 166 5.6 Opening and ﬁlling of nanotubes using chemical methods and capillarity 166 5.6.1 The work of Ajayan and Iijima 166 5.6.2 Selective opening using gas-phase oxidants 167 5.6.3 Opening by treatment with nitric acid 170 5.6.4 Alternative liquid-phase oxidants 172 5.6.5 Filling with molten materials 172 5.6.6 Experiments on capillarity and wetting 173 5.6.7 Chemistry and crystallisation in nanotubes 174 5.6.8 Biological molecules in nanotubes 178 5.7 Filling of single-walled nanotubes 178 5.8 Storing gases in nanotubes 180 5.9 Discussion 181 References 182
6 The ultimate carbon ﬁbre? The mechanical properties of carbon nanotubes 186 6.1 Conventional carbon ﬁbres 187 6.2 Graphite whiskers 188 6.3 Catalytically grown carbon ﬁbres 190 6.4 Mechanical properties of carbon nanotubes 191 6.4.1 Theoretical predictions 191 6.4.2 Experimental observations using TEM: qualitative 192 6.4.3 Experimental observations using TEM: quantitative 196 6.4.4 Experimental observations using scanning probe microscopy 198 6.5 Carbon nanotube composites 200 6.5.1 Introduction 200 6.5.2 Bonding between nanotubes and matrix 202 Contents xi 6.5.3 Aspect ratio 204 6.5.4 Experiments on incorporating nanotubes into a matrix 205 6.5.5 Applications of nanotube-containing composites 206 6.6 Nanotubes as tips for scanning probe microscopes 207 6.7 Discussion 209 References 210
7 Curved crystals, inorganic fullerenes and nanorods 213 7.1 Chrysotile and imogolite 214 7.2 Inorganic fullerenes from layered metal dichalcogenides 218 7.2.1 Synthesis of chalcogenide fullerenes 218 7.2.2 Structure of chalcogenide fullerenes 220 7.2.3 Inorganic fullerenes as solid-state lubricants 222 7.3 Nanotubes and nanoparticles containing boron and nitrogen 223 7.3.1 Boron-carbon-nitride tubes 223 7.3.2 Pure boron nitride tubes and nanoparticles 224 7.3.3 Structure of boron nitride tubes and nanoparticles 226 7.4 Carbide nanorods 229 7.5 Discussion 230 References 232
8 Carbon onions and spheroidal carbon 235 8.1 Carbon onions 235 8.1.1 Discovery 235 8.1.2 Ugarte’s experiments: irradiation of cathodic soot 236 8.1.3 Production of onions from other carbons 237 8.1.4 The structure of carbon onions 239 8.1.5 Formation mechanism of carbon onions 240 8.1.6 Stability of carbon onions 244 8.1.7 Bulk synthesis of carbon onions 244 8.1.8 The formation of diamond inside carbon onions 246 8.2 Spheroidal carbon particles in soot 246 8.2.1 Background 246 8.2.2 Growth mechanisms: the traditional view 248 8.2.3 The icospiral growth mechanism 250 8.2.4 The structure of carbon black 252 8.3 Spherulitic graphite cast iron 254 8.3.1 History 254 8.3.2 The structure of spherulitic graphite 256 8.3.3 The precipitation process 259 xii Contents 8.4 Spheroidal structures in mesophase pitch 260 8.5 Discussion 261 References 262
9 Future directions 266 9.1 Towards a carbon nanotube chemistry 267 9.2 New all-carbon structures 269 9.3 Nanotubes in nanotechnology 270 9.4 Final thoughts 270 References 273
Name index 275 Subject index 277 1 Introduction
Take Carbon for example then What shapely towers it constructs A. M. Sullivan, Atomic Architecture Carbon, in fact, is a singular element . . . Primo Levi, The Periodic Table
The ability of carbon to bond with itself and with other atoms in endlessly varied combinations of chains and rings forms the basis for the sprawling scientiﬁc discipline that is modern organic chemistry. Yet until recently we knew for certain of just two types of all-carbon crystalline structure, the naturally occurring allotropes diamond and graphite. Despite the best eﬀorts of some of the world’s leading synthetic chemists, all attempts to prepare novel forms of molecular or polymeric carbon came to nothing: the elegant all- carbon structures proposed by Roald Hoﬀmann, Orville Chapman and others remained ﬁrmly in the realm of pure speculation. Ultimately, the breakthrough which revolutionised carbon science came not from synthetic organic chemis- try but from experiments on clusters formed by the laser-vaporisation of graphite. Harry Kroto, of the University of Sussex, and Richard Smalley, of Rice University, Houston, had diﬀerent reasons for being interested in the synthesis of carbon clusters. Kroto had been fascinated since the early 1960s in the processes occurring on the surfaces of stars, and believed that experiments on the vaporisation of graphite might provide key insights into these processes. Smalley, on the other hand, had been working for several years on the synthesis of clusters using laser-vaporisation, concentrating chieﬂy on semiconductors such as silicon and gallium arsenide. But he was also interest- ed in what might happen when one vaporises carbon. In August 1985, the two scientists came together at Rice and, with a group of colleagues and students,
1 2 1 Introduction began the now famous series of experiments on the vaporisation of graphite. They were immediately struck by a surprising result. In the distribution of gas-phase carbon clusters, detected by mass spectrometry, C was by far the dominant species. This dominance became even more marked under condi- tions which maximised the amount of time the clusters were ‘annealed’ in the helium. There was no immediately obvious explanation for this since there appeared to be nothing special about open structures containing 60 atoms. The eureka moment came when they realised that a closed cluster containing precisely 60 carbon atoms would have a structure of unique stability and symmetry, as shown in Fig. 1.1. Although they had no direct evidence to support this structure, subsequent work has proved them correct. The dis- covery of C, published in Nature in November 1985 (1.1), had an impact which extended way beyond the conﬁnes of academic chemical physics, and marked the beginning of a new era in carbon science (1.2—1.5). At ﬁrst, however, further progress was slow. The main reason was that the amount of C produced in the Kroto—Smalley experiments was minuscule: ‘a puﬀ in a helium wind’. If C were to become more than a laboratory curiosity, some way must be found to produce it in bulk. Eventually, this was achieved using a technique far simpler than that of Kroto and Smalley. Instead of a high-powered laser, Wolfgang Kra¨tschmer of the Max Planck Institute at Heidelberg, Donald Huﬀman of the University of Arizona and their co- workers used a simple carbon arc to vaporise graphite, again in an atmosphere of helium, and collected the soot which settled on the walls of the vessel (1.6). Dispersing the soot in benzene produced a red solution which could be dried down to produce beautiful plate-like crystals of ‘fullerite’: 90% C and 10% C.Kra¨ tschmer and Huﬀman’s work, published in Nature in 1990, showed that macroscopic amounts of solid C could be made using methods access- ible to any laboratory, and it stimulated a deluge of research. Carbon nanotubes, the primary subject of this book, are perhaps the most important fruits of this research. Discovered by the electron microscopist Sumio Iijima, of the NEC laboratories in Japan, in 1991, these ‘molecular carbon ﬁbres’ consist of tiny cylinders of graphite, closed at each end with caps which contain precisely six pentagonal rings. We can illustrate their structure by considering the two ‘archetypal’ carbon nanotubes which can be formed by cutting a C molecule in half and placing a graphene cylinder between the two halves. Dividing C parallel to one of the three-fold axes results in the zig-zag nanotube shown in Fig. 1.2(a), while bisecting C along one of the ﬁve-fold axes produces the armchair nanotube shown in Fig. 1.2(b). The terms ‘zig-zag’ and ‘armchair’ refer to the arrangement of hexagons around the circumference. There is a third class of structure in which the hexagons are arranged helically 1.1 The discovery of fullerene-related carbon nanotubes 3
Fig. 1.1. C: buckminsterfullerene. around the tube axis (see Chapter 3). Experimentally, the tubes are generally much less perfect than the idealised versions shown in Fig. 1.2, and may be either multilayered or single-layered. Carbon nanotubes have captured the imagination of physicists, chemists and materials scientists alike. Physicists have been attracted to their extraordi- nary electronic properties, chemists to their potential as ‘nanotest-tubes’ and materials scientists to their amazing stiﬀness, strength and resilience. On a more speculative level, nanotechnologists have discussed possible nanotube- based gears and bearings. In this book, an attempt has been made to cover all of the most important areas of nanotube research, as well as discussing related structures such as carbon nanoparticles, carbon onions and ‘inorganic fullerenes’. This opening chapter begins with a brief account of the discovery of carbon nanotubes and then describes some of the basic characteristics of arc-evaporation-synthesised nanotubes. The pre-1991 evidence for the exist- ence of nanotubes is discussed, and some of the directions in which nanotube research is developing are summarised. Finally, the organisation of the book is outlined.
1.1 The discovery of fullerene-related carbon nanotubes Iijima was fascinated by the Kra¨ tschmer—Huﬀman Nature paper, and decided to embark on a detailed TEM study of the soot produced by their technique. He had good reasons for believing that it might contain some interesting structures. Ten years earlier he had studied soot formed in a very similar arc-evaporation apparatus to the one used by Kra¨tschmer and Huﬀman and found a variety of novel carbon architectures including tightly curved, closed 4 1 Introduction
Fig. 1.2. Drawings of the two nanotubes which can be capped by one half of a C molecule (1.7). (a) Zig-zag (9,0) structure, (b) armchair (5,5) structure (see Chapter 3 for explanation of indices). nanoparticles and extended tube-like structures (1.8, 1.9). Might such particles also be present in the K—H soot? Initial high resolution TEM studies were disappointing: the soot collected from the walls of the arc-evaporation vessel appeared almost completely amorphous, with little obvious long-range struc- ture. Eventually, Iijima gave up sifting through the wall soot from the arc- evaporation vessel, and turned his attention to the hard, cylindrical deposit which formed on the graphite cathode after arc-evaporation. Here his eﬀorts were ﬁnally rewarded. Instead of an amorphous mass, the cathodic soot contained a whole range of novel graphitic structures, the most striking of which were long hollow ﬁbres, ﬁner and more perfect than any previously seen. Iijima’s beautiful images of carbon nanotubes, shown ﬁrst at a meeting at Richmond, Virginia in October 1991, and published in Nature a month later (1.10), prompted fullerene scientists the world over to look again at the used graphite cathodes, previously discarded as junk.
1.2 Characteristics of multiwalled nanotubes A typical sample of the nanotube-containing cathodic soot is shown at moder- ate magniﬁcation in Fig. 1.3(a). As can be seen, the nanotubes are accompanied by other material, including nanoparticles (hollow, fullerene-related struc- 1.2 Characteristics of multiwalled nanotubes 5
Fig. 1.3. (a) TEM image of nanotube-containing soot. Scale bar 100 nm. (b) Higher magniﬁcation image of individual tubes. Scale bar 10 nm. tures) and some disordered carbon. The nanotubes range in length from a few tens of nanometres to several micrometres, and in outer diameter from about 2.5 nm to 30 nm. At high resolution the individual layers making up the concentric tubes can be imaged directly, as in Fig. 1.3(b). It is quite frequently observed that the central cavity of a nanotube is traversed by graphitic layers, eﬀectively capping one or more of the inner tubes and reducing the total number of layers in the tube. An example is shown in Fig. 1.4, where a single layer forms a cap across the central tube, reducing the number of concentric layers from six to ﬁve. 6 1 Introduction
Fig. 1.4. High resolution image of multiwalled nanotube with ‘internal cap’. Scale bar 5nm.
Fig. 1.5. Image of typical multiwalled nanotube cap. Scale bar 5 nm.
As mentioned above, virtually all of the tubes are closed at both ends with caps which contain pentagonal carbon rings. In practice, the caps are rarely hemispherical in shape, but can have a variety of morphologies; a typical example is shown in Fig. 1.5. More complex cap structures are often observed, owing to the presence of heptagonal as well as pentagonal carbon rings (1.11). Iijima has often illustrated the role played by pentagonal and heptagonal rings in nanotube caps by referring to the art of Japanese basket-work, of the kind shown in Fig. 1.6, where non-hexagonal rings play a similar topological role. Structures analogous to those of carbon nanotubes also occur among viruses (see Chapter 3), and, perhaps inevitably, among the architectural designs of Buckminster Fuller (Fig. 1.7). 1.3 Single-walled nanotubes 7
Fig. 1.6. Japanese bamboo vase which incorporates pentagonal and heptagonal rings. Courtesy Prof. Eiji Osawa.
1.3 Single-walled nanotubes Nanotubes of the kind described by Iijima in 1991 invariably contain at least two graphitic layers, and generally have inner diameters of around 4 nm. In 1993, Iijima and Toshinari Ichihashi of NEC, and Donald Bethune and colleagues of the IBM Almaden Research Center in California independently reported the synthesis of single-walled nanotubes (1.13, 1.14). This proved to be an extremely important development, since the single-walled tubes ap- peared to have structures which approximate to those of the ‘ideal’ nanotubes shown in Fig. 1.2. Moreover, the single-walled tubes were completely novel. While multiwalled graphitic tubules, produced by catalysis, had been known for many years before the discovery of fullerene-related nanotubes (see next section), nothing like single-walled carbon nanotubes had been observed before. An early image of a single-walled nanotube (SWNT) sample is shown in Fig. 1.8(a). It can be seen that the appearance is quite diﬀerent to that of samples of multiwalled nanotubes (MWNT). The individual tubes have very small diameters (typically : 1 nm), and are curled and looped rather than straight. In this image, the tubes are contaminated with amorphous carbon and catalytic particles; subsequent work has enabled much purer samples to be produced. A higher magniﬁcation image of some individual tubes is shown in Fig. 1.8(b). Fig. 1.7. The original ‘buckytube’? Buckminster Fuller’s design for the entrance pavilion of the Union Tank Car Company dome, Baton Rouge, Louisiana (1.12). 1.3 Single-walled nanotubes 9
Fig. 1.8. Typical sample of single-walled nanotubes. (a) General area, showing tubes coated with amorphous carbon. Catalytic metal particles can also be seen (courtesy Donald Bethune). (b) Higher magniﬁcation image of individual tubes (1.15).
An alternative method of preparing single-walled nanotubes was described by Smalley’s group in 1996 (1.16). Like the original method of preparing C, this involved the laser-vaporisation of graphite, and resulted in a high yield of single-walled tubes with unusually uniform diameters. These highly uniform tubes had a greater tendency to form aligned bundles than those prepared using arc-evaporation, and led Smalley to christen the bundles nanotube ‘ropes’. Initial experiments indicated that the rope samples contained a very high proportion of nanotubes with a speciﬁc armchair structure. This created 10 1 Introduction considerable excitement (1.17), since one of the problems with nanotube samples up to that point was the wide range of diﬀerent structures present. Subsequent work has suggested that the rope samples may be less homogene- ous than originally thought. Nevertheless, the synthesis of nanotube ropes gave an important boost to nanotube research, and some of the most impres- sive work has been carried out on these samples.
1.4 Pre-1991 evidence for carbon nanotubes The discovery of carbon nanotubes was immediately recognised as an import- ant event, and prompted the question: why were they not discovered many years ago? The same question has frequently been asked about buckminster- fullerene itself. All of the techniques required to prepare and characterise these materials have been available for decades, so why did we have to wait so long? In the case of carbon nanotubes, part of the answer seems to be that they were seen previously, but simply not recognised as a new and important form of carbon. From a historical point of view it is of interest to review the pre-1991 evidence for the existence of ‘buckytubes’, but this should not be seen as diminishing the importance of Iijima’s work, which was the ﬁrst to appreciate fully the nature and importance of these structures. A letter in Nature in October 1992 claimed that nanotubes had been observed as early as 1953 (1.18). The writer described thread-like carbon structures obtained from the reaction of CO and FeO at 450 °C, which he suggested were ‘similar, if not identical’ to carbon nanotubes. This illustrates the care which must be taken in assessing claims of prior discovery in this area. Fine tubules of carbon produced by catalytic methods have been known for many years, but these have a much less perfect structure than the fullerene- related tubes, as discussed in Chapters 2 and 3. The tubes are not closed with fullerene-like caps, but usually have a metal particle attached to one end. Although there has been a substantial amount of research on carbon tubules produced by catalysis (e.g. 1.19), these imperfect structures do not lend them- selves to the range of potential applications which seem possible for fullerene- related nanotubes. A number of authors have also pointed out the similarities between carbon nanotubes and graphite whiskers, the highly perfect form of carbon ﬁbres which were ﬁrst prepared by Roger Bacon in 1960 (1.20). It is certainly true that the technique used to produce whiskers, which involves a DC carbon arc, seems very close to the arc-evaporation method of nanotube synthesis. How- ever, there are major diﬀerences between graphite whiskers and carbon nanotubes, not least the fact that whiskers are far larger: typically about 5 lm 1.4 Pre-1991 evidence for carbon nanotubes 11 in diameter and up to 3 cm in length. There are also structural diﬀerences: whiskers are scroll-like, while nanotubes are believed to have Russian-doll like structures (see Chapter 6 for further details on whiskers). If catalytically produced tubes and graphite whiskers can be dismissed, what is the evidence that genuine carbon nanotubes were observed prior to 1991? To begin, there are Iijima’s studies of carbon ﬁlms carried out in the late 1970s and early 1980s, which were mentioned above. For this work he prepared speci- mens of arc-evaporated carbon using an apparatus of the type commonly employed to make carbon support ﬁlms for electron microscopy. The method he used would have diﬀered slightly (but signiﬁcantly) from the Kra¨t- schmer—Huﬀman technique in that the chamber would have been evacuated rather than ﬁlled with a small pressure of helium. The resulting ﬁlms were largely amorphous, but contained small, partially graphitized regions which contained some unusual structures. These structures included discrete graph- itic particles apparently made up of concentric closed shells, tightly curved around a central cavity. One of these structures, reproduced as Figure 5(a) in his 1980 Journal of Microscopy paper (1.8), is clearly a nanotube, and Iijima conﬁrmed its tubular nature using tilting experiments. But he did not explore these structures in detail, and suggested that the curved layers were probably due to sp bonding, rather than, as we now believe, the presence of pentagonal rings. There are other examples of nanotube-like structures scattered throughout the pre-1991 carbon literature (see, for instance, Fig. 10 in Ref. (1.21)). In some cases these structures might be contaminants on the carbon ﬁlms used to support the samples (see p. 34). Evidence for the existence of elongated fullerene-like structures also came from high resolution electron microscopy studies of C crystals. In one of the ﬁrst such studies, published in July 1991 (1.22), Su Wang and Peter Buseck of Arizona State University reported that fullerite crystals contained closed carbon cages both smaller and larger than C. The larger fullerenes had the projected shapes of elongated ellipsoids, which were estimated to contain roughly 130 carbon atoms. It is possible that such structures arose from the coalescence of adjacent C or C molecules in the crystal. Work by other authors also anticipated the discovery of carbon nanotubes. For example, Patrick Fowler of Exeter University described theoretical studies of small cylindrical fullerene molecules in early 1990 (1.23). Two groups of American theoreticians, one at the Naval Research Laboratory, Washington DC (1.24), and one at the Massachusetts Institute of Technology (1.25) submit- ted papers on the electronic properties of fullerene tubes just a few weeks before Iijima’s paper appeared in Nature. Finally, the highly imaginative 12 1 Introduction British chemist David Jones, under his pen-name Daedalus, also ruminated about rolled-up tubes of graphite in the New Scientist in 1986 (1.26). He suggested that molecules of this type might behave as extremely viscous supercritical gases at room temperature, which could be useful in calming the atmosphere at violent public demonstrations. Although this particular proph- ecy did not prove accurate, Daedalus has an excellent record in the ﬁeld of fullerene research. In the 1960s he had predicted the existence of spherical carbon molecules, anticipating the discovery of fullerenes by nearly 20 years.
1.5 Nanotube research The method for producing nanotubes described by Iijima in 1991 gave rela- tively poor yields, making further research into their structure and properties diﬃcult. A signiﬁcant advance came in July 1992 when Thomas Ebbesen and Pulickel Ajayan, working at the same Japanese laboratory as Iijima, described a method for making gram quantities of nanotubes (1.27). Again, this was a serendipitous discovery: Ebbesen and Ajayan had been trying to make fullerene derivatives when they found that increasing the pressure of helium in the arc-evaporation chamber dramatically improved the yield of nanotubes formed in the cathodic soot. The availability of nanotubes in bulk gave an enormous boost to the pace of research worldwide. One area which attracted early interest was the idea of using carbon nanotubes and nanoparticles as ‘molecular containers’. A landmark in this ﬁeld was the demonstration, by Ajayan and Iijima, that nanotubes could be ﬁlled with molten lead, and thus be used as moulds for ‘nanowires’ (1.28). Subsequently, more controlled methods of opening and ﬁlling nanotubes have been developed, enabling a wide range of materials, including biological ones, to be placed inside. The resulting opened or ﬁlled tubes might have fascinating properties, with possible applications in catalysis, or as biological sensors. Filled carbon nanoparticles may also have important applications, in areas as diverse as magnetic recording and nuclear medicine. Perhaps the largest volume of research into nanotubes has been devoted to their electronic properties. The theoretical work which pre-dated Iijima’s discovery has already been mentioned. A short time after the publication of Iijima’s 1991 letter in Nature, two other papers appeared on the electronic structure of carbon nanotubes (1.29, 1.30). The MIT group, and Noriaki Hamada and colleagues from Iijima’s laboratory in Tsukuba, carried out band structure calculations on narrow tubes using a tight-binding model, and demonstrated that electronic properties were a function of both tube structure and diameter. These remarkable predictions stimulated a great deal of interest, 1.6 Organisation of the book 13 but attempting to determine the electronic properties of nanotubes experimen- tally presented great diﬃculties. Since 1996, however, experimental measure- ments have been carried out on individual nanotubes, which appear to conﬁrm the theoretical predictions. These results have prompted speculation that nanotubes might become components of future nanoelectronic devices. Determining the mechanical properties of carbon nanotubes also presented formidable diﬃculties, but once again experimentalists have proved equal to the challenge. Measurements carried out using transmission electron micro- scopy and atomic force microscopy have demonstrated that the mechanical characteristics of carbon nanotubes may be just as exceptional as their elec- tronic properties. As a result, there is growing interest in using nanotubes in composite materials. A variety of other possible applications of nanotubes are currently exciting interest. For example, a number of groups are exploring the idea of using nanotubes as tips for scanning probe microscopy. With their elongated shapes, pointed caps and high stiﬀness, nanotubes would appear to be ideally suited for this purpose, and initial experiments in this area have produced some extremely impressive results. Nanotubes have also been shown to have useful ﬁeld emission properties, which might lead to their being used in ﬂat-panel displays. Overall, the volume of nanotube research is growing at an astonish- ing rate, and commercial applications will surely not be far behind.
1.6 Organisation of the book The chapter which follows considers the various methods for synthesising nanotubes, including catalytically produced and single-walled tubes, and sum- marises current thinking on growth mechanisms. Methods of purifying, align- ing and processing nanotubes are also covered. In Chapter 3, theoretical approaches to the analysis of nanotube structure are outlined, and experimen- tal observations described. The structures of carbon nanoparticles and nanocones are also discussed. Chapter 4, entitled ‘The physics of nanotubes’, is primarily concerned with the electronic properties of carbon nanotubes, but also considers magnetic, optical and vibrational properties of nanotubes, as well as experimental studies of nanotubes as ﬁeld emitters. Methods of opening and ﬁlling carbon nanotubes and nanoparticles are described in Chapter 5, together with the possible uses of these ﬁlled nanocapsules. Theoretical and experimental work on the mechanical properties of nanotubes, and nanotube- containing composites are discussed in Chapter 6. Chapter 7 covers inorganic analogues of fullerenes and nanotubes. Curved and tubular inorganic crystals have been known for many years, but there has 14 1 Introduction been renewed interest in such structures since the discovery of ‘inorganic fullerenes’ based on dichalcogenides by Israeli workers in 1992. Fullerene-like structures containing boron and nitrogen are also discussed in this chapter. In Chapter 8 a discussion is given of spheroidal forms of carbon. The ﬁrst part of the chapter is concerned with the recently discovered fullerene-like structures known as ‘onions’, and this is followed by a brief survey of more well estab- lished spheroidal carbon structures including soot and carbon black particles. The evidence that these structures contain fullerene-like elements is reviewed. Finally, Chapter 9 considers some possible future directions in which nanotube science might develop.
(1.1) H. W. Kroto, J. R. Heath, S. C. O’Brien, R. F. Curl and R. E. Smalley, ‘C: Buckminsterfullerene’, Nature, 318, 162 (1985). (1.2) J. Baggott, Perfect symmetry: the accidental discovery of buckminsterfullerene, Oxford University Press, 1994. (1.3) H. Aldersey-Williams, The most beautiful molecule, Aurum Press, London, 1995. (1.4) H. W. Kroto, ‘Symmetry, space, stars and C’ (Nobel lecture), Rev. Mod. Phys., 69, 703 (1997). (1.5) R. E. Smalley, ‘Discovering the fullerenes’ (Nobel lecture), Rev. Mod. Phys., 69, 723 (1997). (1.6) W. Kra¨tschmer, L. D. Lamb, K. Fostiropoulos and D. R. Huﬀman, ‘Solid C: a new form of carbon’, Nature, 347, 354 (1990). (1.7) M. Ge and K. Sattler, ‘Scanning tunnelling microscopy of single-shell nanotubes of carbon’, Appl. Phys. Lett., 65, 2284 (1994). (1.8) S. Iijima, ‘High resolution electron microscopy of some carbonaceous materials’, J. Microscopy, 119, 99 (1980). (1.9) S. Iijima, ‘Direct observation of the tetrahedral bonding in graphitized carbon black by high-resolution electron microscopy’, J. Cryst. Growth, 50, 675 (1980). (1.10) S. Iijima, ‘Helical microtubules of graphitic carbon’, Nature, 354, 56 (1991). (1.11) S. Iijima, T. Ichihashi and Y. Ando, ‘Pentagons, heptagons and negative curvature in graphitic microtubule growth’, Nature, 356, 776 (1992). (1.12) J. Ward, ed., The artifacts of Buckminster Fuller, Vol. 3, Garland Publishing, New York, 1985. (1.13) S. Iijima and T. Ichihashi, ‘Single-shell carbon nanotubes of 1-nm diameter’, Nature, 363, 603 (1993). (1.14) D. S. Bethune, C. H. Kiang, M. S. de Vries, G. Gorman, R. Savoy, J. Vasquez and R. Beyers, ‘Cobalt-catalysed growth of carbon nanotubes with single-atomic-layer walls’, Nature, 363, 605 (1993). (1.15) C. H. Kiang, P. H. M. van Loosdrecht, R. Beyers, J. R. Salem, D. S. Bethune, W. A. Goddard III, H. C. Dorn, P. Burbank and S. Stevenson, ‘Novel structures from arc-vaporized carbon and metals: single-layer nanotubes and metallofullerenes’, Surf. Rev. Lett., 3, 765 (1996). (1.16) A. Thess, R. Lee, P. Nikolaev, H. Dai, P. Petit, J. Robert, C. Xu, Y. H. Lee, S. G. Kim, A. G. Rinzler, D. T. Colbert, G. E. Scuseria, D. Toma´ nek, J. E. References 15
Fischer and R. E. Smalley, ‘Crystalline ropes of metallic carbon nanotubes’, Science, 273, 483 (1996). (1.17) P. Ball, ‘The perfect nanotube’, Nature, 382, 207 (1996). (1.18) J. A. E. Gibson, ‘Early nanotubes?’, Nature, 359, 369 (1992). (1.19) R. T. K. Baker and P. S. Harris, ‘The formation of ﬁlamentous carbon’, Chem. Phys. Carbon, 14, 83 (1978). (1.20) R. Bacon, ‘Growth, structure and properties of graphite whiskers’, J. Appl. Phys., 31, 283 (1960). (1.21) G. R. Millward and D. A. Jeﬀerson, ‘Lattice resolution of carbons by electron microscopy’, Chem. Phys. Carbon, 14, 1 (1978). (1.22) S. Wang and P. R. Buseck, ‘Packing of C molecules and related fullerenes in crystals: a direct view’, Chem. Phys. Lett., 182, 1 (1991). (1.23) P. W. Fowler, ‘Carbon cylinders: a new class of closed-shell clusters’, J. Chem. Soc., Faraday Trans., 86, 2073 (1990). (1.24) J. W. Mintmire, B. I. Dunlap and C. T. White, ‘Are fullerene tubules metallic?’, Phys. Rev. Lett., 68, 631 (1992). (1.25) M. S. Dresselhaus, G. Dresselhaus and R. Saito, ‘Carbon ﬁbers based on C and their symmetry’, Phys. Rev. B, 45, 6234 (1992). (1.26) D. E. H. Jones (Daedalus), New Scientist, 110 (1505), 88 and (1506), 80 (1986). (1.27) T. W. Ebbesen and P. M. Ajayan, ‘Large-scale synthesis of carbon nanotubes’ Nature, 358, 220 (1992). (1.28) P. M. Ajayan and S. Iijima, ‘Capillarity-induced ﬁlling of carbon nanotubes’, Nature, 361, 333 (1993). (1.29) R. Saito, M. Fujita, G. Dresselhaus and M. S. Dresselhaus, ‘Electronic structure of graphene tubules based on C’, Phys. Rev. B, 46, 1804 (1992). (1.30) N. Hamada, S. Sawada and A. Oshiyama, ‘New one-dimensional conductors: graphitic microtubules’, Phys. Rev. Lett., 68, 1579 (1992).